IS : 5491-1969
CODE OF PRACTICE FOR
LAYING IN SITUGRANOLTTHIC CONCRETE
( Fourth Reprint JUNE 1990)
@ CoPyright 1970
BUREAU OF INDIAN STANDARDS
MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARG
NEW DELHI 110002
Gr 4 Augusf 1970
( Reaffirmed 1996 )
IS : 5491- 1969
CODE OF PRACTI-CE FOR
LAYING IN SITU GRANOLITHIC CONCRETE
Flooring and Plastering Sectional Committee, BDC 5
SHRI M. S. BHATU Central Public Works Department
DR D. BANVRJEE Nawttbber Manufacturers Ltd, CalcutLa
DR M. L. BHAUMIK -3
SHXI DINESH_A,M~I Arcoy Industries, Ahmedabad
SHRI RAS~KLALA. CIIOKS~I ( Altcrnn~c)
DEPUTY CHILF MECHANICAL Ministry of Railways
ENOINXEI(, INTEQRAL COAC)~
DEPDTY DIRECTOR ( AXCH ),
TION, LU~KNOW ( Alternate )
SHRI P. K. Docxon The Concrete Association of India, Bombay
SHRZ K. P. GHOSH Engineer-in-Chief’s Branch, Army Headquarters
SI~RI B. P. MIJKNI~XJEIX( Alternate)
SHRI N. HARILAI. Oxy=&oride Flooring Products Ltd, Bombay
Dn PI~ANLALPATXL ( Alternate )
DR JOSEPII G~oltce Central Building ‘Research Institute ( CSIR ), Roorkee
Da MOHAN RAI ( Alternate )
SHIZIS. C. KAPOOR Modern Tiles & Marble, New Delhi
SHRI A. C. KAPOOIZ( Alfnnatc)
SHRI M. R. MALYA Burmah-Shell Oil Storage & Distributing Co of India
Da B. S. BASSI (Alternate )
SHRI HAZARI LAL MARWAH Central Builders’ Association, New Delhi
SHRI T. R. MEIIANDRU The Institution of Engineers ( India ), Calcutta
SHRI M. V. MURUGAPPAN Coromandel Prodorite Pvt Ltd, Madras
SHRI Ii. SRINIVASAN ( Alternate )
SHRI H. M. NANDKEOLYAR Indian Linoleums Ltd,_24 Parganas ( West Bengal )
SHRI M. G. PADRYE Maharashtra Engineering Research Institute, Nasik
SHRI N. M. Joa ( Alternate)
SHRI RAGMANM. PATEL The Bhor Industries Ltd, Bombay
SHRI J. M. SHKOFF (Alternate)
SHRI RXBINDER SINGII National Buildings Organization, New Delhi
Sn nr 0. P. RATRA ( Altcrnafe )
( Continued on page 2 )
BUREAU OF INDIAN STANDARDS
MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARG
NEW DELHI 110002
IS : 5491-1969
(Continued from page 1 )
S-rlnr E. K. RA&~ACZIANDRAN National Test House, Calcutta
SIIRI K. L. nANRR.TRR (Altcrnafe )
SHRI G. S. SAvKAu Directorate General of Supplies & Disposals
Srrar L. G. SELVAI Bureau of Public Enterprises ( Ministry of Finance )
&tar T. M. VARUQHXSE ( Alternate )
SI~RI G. C. SHAIMA Indian Institute of Architects, Bombay
( PLANNINO AND
ENCIN~~ Publkadorks Department, Government of Tamil
DEPUTY CIXIXF ENOINEER
( BUILDINCJ ) ( Affernate )
SUPERINTENDINR Suuvvxo~ OF Central Public Works Department, New Delhi
SURVEYOR OF WORKS 1 TO
SSV I (Alternate )
SHRI R. NA~ARAJAN,
Director ( Civ Engg )
Director General, ISI ( Ex-o&cio Member)
SHRX L. RABIACIIANDRARno
Deputy Director (Civ Engg), IS1
Panel for Laying in sifu Granolithic Concrete Floor
Topping, BDC 5:P3
SHR~ L. G. SELVAM
1. Bureau of Public Enterprises ( Ministry oP Finance )
DR S. M. K. CIIETTY Central Building Research Institute ( CSIR ),
SHRI K. P. GHOSH In personal capacity ( D-25, Hauz Khas, .New Delhi 16)
Snnr K. G. RASA~OPALAN Central Public Works Department, New Delhi
IS : 5491-1969
CODE OF PRACTICE FOR
LAYlNG IN SZTU GRANOLITHIC CONCRETE
0.1This Indian Standard was adopted by the Indian Standards Institution
on 23 October 1969, after the draft finalized by the Flooring and Plaster-
ing Sectional Committee had been approved by the Civil Engineering
0.2 Granolithic concrete floor topping is adopted for floors of heavy
engineering-factories, workshops, garrages, warehouses, etc, where the floor
is subjected to heavy loads, and severe abrasion combined with impact.
The granolithic concrete essentially consists of a rich concrete made with
specially selected aggregate of ‘high hardness, surface texture and particle
shape suitable for use as a wearing finish to floors. Although plain
concrete as laid conforming to IS,:2571-1963* would be satisfactory for
many purposes, granolithic concrete is chosen because of its high abrasion
resistance and used for floor toppiygs wherever abrasion combined with
impact is likely to be severe. In this standard the method of laying the
granolithic concrete topping is only given and all other details up to the
laying of base concrete or suspended slab shall conform to the procedure
laid down in IS : 2571-1963* which is an adjunct to this standard.
0.3 There are two methods of laying the in situ granolithic concrete floor
topping. The topping shall either be laid within three hours of the laying
of the base, that is, monolithically with the base concrete; or alternatively,
it shall be laid at any time after the base had begun to harden, in such a
way as to produce the maximum possible bond between the base and top-
ping, that is, it shall be laid separately from the base. A high standard of
workmanship is essential and skilled floor layers should be employed for the
job. Inferior work often leads to curling, breaking of bond between the
base and topping concrete, cracking and dusting of the top surface. .In
ground floors, it is advisable to lay the granolithic concrete topping monoli-
thically with the base concrete. Depending upon the nature of use and
performance expected from the floor topping, the floor finish has to be laid
*Code of practice for laying in situ cement concrete flowing ( Since revised ).
IS : 5491- 1969
ill varinus /hicknesses and a careful sclcction has to he made regarding mix
prnpc)rtio;!s, p:~n~il sizes a11cl the type of co::struction. This cotlc has I)et:n
prepar~~~l M.itll a :ielv to providing the necessary guidance ill tlte selection
of matWi:tli, method of laying and finishing of granolithic concrete
topping for ol)tninillg sntisfkctory performance of the flooring.
0.4 In the formulation of this standard due wcightagc has been given to
international co-nrdination among the standards and practices prrvailillg
in different countries in addition to relating it to the practices in the lkltl III
this country. This has been met by derivin, 0‘ assistance from the following
puljlications published by the British Standards Institution:
B.S.CP 204: 1965 In situ floor finishes.
B.S. 882 and 1201 : 1965 Aggregates from natural sources for concrete
( including granolithic ).
0.5 For the purpose of deciding whether a particular requirement of this
standard is complied with, the final value, observed or calculatcct, express-
ing the result of a test, shall be rounded off in accordance with IS : 2-l%O*.
The number of significant places retained in the rounded off value shculd
be the same as that of the specified value in this standard.
1.1 This standard relates to the laying of granolithic concrete floor topping
laid if2 situ.
2.0 For the purpose of this standard, the definitions given in IS:2j71-
19637 and the following shall apply.
2.1 Base Cpncrete-The layer of concrete on which the granolithic
cdnc.ete floor topping is laid.
2.2 Granolithic Concrete-Concrete made with specially s*lected
aggregate of high hardness, surlicc texture and particle shop:: suitable fol
use as n xvearing finish to floors.
2.3 Surface Hardener-A substance ~vhich may be applied to the surface
of hardened concrete to incrcnse the wear resistance of the concrete.
*Ilules fov rounding off numerical values ( rcuisrd).
tCodc of practice for hying i/l sifu cement concrete flooring ( Since revised ).
IS l 5491~11969.
3.1 Cement-Cement used shall conform to IS:269-1967* or IS:455-
1962t or IS: 1489-1967:.
3.2.1 The aggregates for granolithic concrete floor topping shall consist
of crushed rock of one or more of the following groups:
a) Granite, b) Basalt, c) Trap, and d) Quartzite.
The aggregate shall conform to the requirements of IS: 383-19635.
The aggregate crushing value, when determined in accordance with
IS:2386 (Part IV)-196311, shall not exceed 30 percent. The grading of
the aggregates for granolithic concrete floor topping shall conform to
Tables 1 and 2.
3.2.111 &rrse aggregate -The grading of coarse aggregate for grano-
lithic concrete floor topping shall be within the limits given in Table 1.
TABLE 1 COARSE AGGREGATE
IS SIEVE DESIGNATION PERCENTAQE BY WEIGHT PASSINGIS SIEVES
12.5~mm 90 to 100
IO-mm 40 to 85
4*75-mm 0 to 10
22.214.171.124 Fine aggregate-The grading of fine aggregate for granolithic
concrete floor topping shall be within the limits of one of the two zones
given in Table 2. The fine aggregate shall be described as fine aggregate
of the grading zone into which it falls.
3.3 Water--Water used shall be clean and free from oil, acid, alkali, l
organic or vegetable matter. Sea water shall not be used. Generally
potable water will be suitable.
*Specification for ordinary, rapid hardening and low heat portland cement (second
rerrision). ( S+tcr revised ).
TSpecification for portland blast furnace slag cement (reuiscd). Since reviscd.
$pecification for portland pozzolana cement (wised).
gspecification for coarse and fine aggregates from natural sources for concrete
( ,euisPd ).
l/Methods of test for aggregates for concrete : Part IV Mechanical properties.
IS : 5491.1969
TABLE 2 FINE AGGREGATE
( Clause 126.96.36.199 )
IS SIEVE DESIGNATION PERCENTAQF,BY WEIGTIT
PASSING IS SIEVES
Grading Zone 1 Grading Zone 2
90 to 100 90 to 100
60 ,, 95 75 ), 100
30 70 55 90,, ,,
15 34 35 ,) 59))
5 20 8 ,, 30,,
0 ,, 10 0 1, 10
3.4 Admixtures - Integral additions, either as hardeners or accelerators,
or other surface hardening treatments are not normally required, but their
application may be advantageous in certain circumstances. Caution
should be exercised in the use of admixtures and the manufacturer’s
recommendations should be followed wherever required.
3.5 Abrasives-Metallic or non-metallic materials of high abrasion resis-
tance may be incorporated in the floor topping mix to increase the
abrasion resistance of the floor topping.
3.6, Surface Hardening Solutions - These may be solutions of sodium
silicate, magnesium silicofluoride, or zinc silicofluoride or proprietary
materials consisting mainly of one or more of these compounds. Proprietary
materials may be used only in accordance with the manufacturer’s
instructions ( see Appendix A).
4. DESIGN CONSIDERATIONS
4.1 Abrasion Resistance -- Although plain concrete is ssitisfactory for
many purposes, granolithic concrete has higher abrasion resistance and
should be used for floor topping wherever abrasion is likely to be severe.
4.2 Size of Panels-The floor topping shall be divided into suitable
panels so as to reduce the risk of cracking. Size of the panel is governed
by the thickness of floor finish, the type of construction (monolithic or
separate), local conditions of temperature, humidity and the season in
which flooring is laid. For floor finish laid in exposed situations or in hot
and dry climates, the size of the panels shall be smaller as compared to the
floor finish laid in less exposed situations or in cold and humid climates;
-IS : 5491- 1969
the size of panels laid monolithically with the base may be larger than
that of floor finish laid separately on the hardened base. Generally, in the
case of suspended slabs no dimension of a panel shall exceed 4 m
in case of floor topping laid monolithically with the structural slab and 2 m
iit case of floor topping laid separately on a hardened base. In case
of ground floors, the size of the topping panel may synchronize w~ith
that of the base concrete. Length of a panel shall not exceed one and a
half times its breadth.
4.3 Joints- Construction joints between bays of the floor finish need only
be plain untreated vertical butt joints and should be placed over any
joints in the base.
Where expansion joints are necessary in the walls and roof of a
building, there should be corresponding joints in the floor. The floor
finish should not be allowed to cover the joint filler of the expansion joint
in the base concrete; either the joint filler should extend through the
full thickness of the base concrete and finish or the space above it should
be filled with a suitable sealing compound.
4.4 Mix Proportions-Mix proportion for the granolithic concrete floor
topping for different types of floor finish shall be 1: 1:2 (cement: fine
aggregate : coarse aggregate, by volume ).
4.5 Protection Against Dampness -The layer of coarse sand or
boulder soling provided under the base concrete will generally serve the
~purpose of damp-proofing required for ordinary floors under normal
conditions. However, in more severe conditions, where it is expected
that the dampness may find its way on the top of the floor in the course of
usage of floor, a more effective damp-proof treatment shall be given
underneath the floor by either of the methods given below:
a) Laying the base concrete in two layers and painting the top of the
lower layer with two coats of bitumen conforming to. IS: 1580-
1969* applied at the rate of 1.5 kg/ma, The surface of the lower
layer shall be finished smooth while laying the concrete so that
bitumen can be applied uniformly. The bnumen shall be applied
after the concrete has set and is sufficiently hard.
b) Sandwiching a waterproofing membrane, such as bitumen felt
conlorming to IS: 1322-19657 in the base concrete laid in two
layers. The surface of the lower layer shall be finished smooth
while laying the concrete so as to provide an even surface and
thus prevent damage to the surface of waterproofing membrane.
*Specification for bituminous compounds for waterproofing and caulking purposes
tSpecification for bitumen felts for waterproofing and damp-proofing ( rezkeci). Since
IS : 5491- 1969
4.5.1 1lihele it is expected that the dampness may find its way from the
surrounding walls, the same shall also be elfectively damp-proofed up to
at least 150 mm above the level of the base or sub-floor, anti the damp-
proof treatment below the floor shall be cxtendcd over the walls. Base-
ment floors shall be damp-proofed according to rccommcndatious of
5. COMPACTION EQUIPMENT .
5.1 Compacting Plaxit- The tampers used shall be capal)le of compact-
ing the full thickness of each layer of concrctc and of producing the
desired surface finish. The following types of compactor may be used:
a) Hand tamper having a tamping edge shod with steel strip 75 mm
wide fixed to the tamper by countersunk screws.
b) Hand tamper to which are attached vibrating units operated
either electrically or by an internal combustion engine.
c) Pneumatic tamper in which pneumatic hammers operate on
a steel plate.
d) Pan vibrator.
6. LAYING FLOOR TOPPING OVER BASE CONCRETE
6.1 Floor Topping Laid Monolithically with the Base Concrete (see
Table 3 )-On the clean, green surface of the base concrete laid in
accordance with the procedure given in IS: 2571-1963T the topping shall
be placed in position as soon as possible but generally not later than two to
three hours of laying the base concrete, depending upon the temperature
and the atmospheric conditions. The base concrete at the time of laying
the topping shall be still green but sufficiently firm to enable the workmen
to work over it by placing planks on its surface. The granolithic concrete
mix ( 1: 1:2) for the topping shall be deposited on the base concrete in
the screed strips already laid and thoroughly compacted to the finished
thickness. The surface shall be tested with a straightedge and mason’s
spirit-level to detect any undulation in the surface which, if any, shall be
made good immediately. The topping shall then be floated with a
wooden float to render the surface even and after the surface is slightly
hardened, it shall be finished smooth as described in IS :257 l-1963?.
6.2 Floor Topping Laid Separately on Hardened Base Concrete ( see
Table 3)-Before the operation for laying the topping is started, the
surface of base concrete shall be thoroughly cleaned of all dirt, loose
particles, caked mortar droppings, and laitance, if any, by scrubbing with
coir or steel wire brush. Where the concrete has hardened so much that
*Code of practice for laying damp-proof treatment using bitumen felts (revised ).
tCode of practice for laying in situ cement concrete flooring. ,‘Sinm r,,,,~ed.
IS : 5491- 1969
roughening bf surface by wire I~id~ is not possible, the w~lhx shall be
rougllcnrd by chipping or hflckillg at clost- intervals. Ueltirc laying the
topping, the surface shall be wetted widr water for several hours and
surp111s water shall be removed .l)y mopping immediately before the
topping is laid in position.
The screed strips shall be fixt~l over the base concrete dividing it into
suitable panels as recommended in 4.2. The screed strips shall be so
arranged that the joints, if any, in the base concrete shall coincide with the
joints in the topping. Before placing the granolithic concrete mix ( 1 : 1 : 2 )
for topping, neat cement slurry shall be thoroughly brushed into the
prepared surface of the base concrete. The topping shall be laid in
accordance with 6.1, very thoroughly tamped, struck off level and the
surface floated with a wooden float. The top surface of the granolithic
concrete shall be tested tvith the straightedge and mason’s spiritilevel
to detect any inequalities in the surface which, if any, shall be made good
immediately. The top surface shall be finished smooth as described
in IS: 2571-1963*.
7. LAYING FLOOR TOPPING ON SUSPENDED SLABS
7.1 Floor Topping Laid Monolithically with the Suspended Slab ( see
Table 3).-The form-work for suspended slab shall bc erected to the
finidd thickness of floor finish. Structural concrete shall be dellasited
in the forms, thoroughly consolidated and surface finished below the
top edge of the form to accommodate the required thickness of the topping.
Any slope required in the floor finish shall be given in the structural
concrete itself, and any laitance or scum shall be brushed away from the
surface of concrete when it is still green. The surface shall not be
finished smooth but kept rough to provide an adequate ~WWI fbr the
On the green surface of the structural concrete, granolithic concrete
( 1 : 1 : 2) shall be placed in position immediately after the structural
concrete has stiffened enough (but his still plastic ) to allow for the
workmen to tread over it by placing planks. Laitance and foreign
matter, if any, shall be removed before the granolithic concrete topping is
placed in posit&n. The topping shall be thoroughly compacted and
screcded to the finished grade. The mix for the structural concrete
as well as the topping shall be as sti8as posiible consistent with workahilit)
so as to prevent accumulation of excess of water or laitsncc: on the
surface. ‘The topping shall theri be floated with a wooden float to rc&er
*Code of~practicc for laying i-~ situ crnwnr concrete flooring. ( Since revised ).
IS : 5491- 1969
the surface even. After the surface is slightly hardened, it shall be finished
in accordance with 6.1.
NATE 1 - In the monolithic methorl of construction the granolilhic concrete floor
topping may be regarded as contributing to the structural strength of the suspended
NOTE 2 -The monolithic construction of granolithic concrete Iloor topping
presents certain difficulties in construction due to other activities, such as plastering
of walls and ceilings, fixing of joinery, movement of scafthldings, Iatl~!ers, etc, which
are likely to damage the floor finish.
7.2 Floor Topping Laid Over the Hardened Suspended Slab (see
Table 3 )-When the topping is to he laid sepnrately over the suspended
slab, the slab shall bc thoroughly brushed with a coil- or steel wire brush
to remove any scum or laitance and swept clean to expose the coarse
aggregates arid leave the surface rough. Where the concrete has hardened
so much that roughening of surface by wire brush is not possible, the
surface shall be roughened by chipping or hacking at close intervals.
Before layi:lg the topping, the surface of the slob shill be wetted with
water for several hours 2nd surplus water shall be removed by mopping
immediately before the topping is laid in position.
The screed strips shall then be fixed over the suspended slab dividing
it into suitable panels as recommended ill 4.2. Immediately before
depositing the granolithic concrete ( 1 : 1: 2 ) for the topping, neat cement
slurry shall be thzn-oughly brushed into the ~prepared surface of the
suspended slab. The granolithic concrete topping shzll be then laid
in accordance with 6.2, thoroughly tamped struck off level and surface
floated with wooden float. The surface shall then be tested with a
straightedge an4 mason’s spirit-level to detect any inequalities and
undulations in subface which, if any, shall be made good immediately.
The top surface shall be finished smooth.
7.3 Floor Topping Laid Over Cushioning Layer (see Table 3) -
Before laying the cushioning lime concrete (see Note), the surface of
the suspended slab shall be prepared as in 7.2. On the clean damp surface
of the suspended slab, lime concrete shall be evenly spread between forms,
thoroughly tamp?d and levelled. Lime concrete shall be prepared
in accordance with IS: 2541-1965*.
Before laying the granolithic concrete topping, the surface of
lime concrete shall be thoroughly clean and prepared as recommended
for base concrete in 6.2. Immediately before spreading the granolithic
concrete ( 1: 1 : 2) for topping, the surface shall be brushed with a thin
layer of neat cement slurry. The granolithic concrete shall then be laid
and finished smooth as given in 6.2.
NOTE- Where lime and good quality of bricks are not available 1: 4.8 cement
concrete may be used. I
*Code of practice for use of lime concrete in buildings.,Since revised.
IS : 5491.1969
TABLE 3 DIFFERENT TYPES OF GRANOLITHIC
CONCRETE FLOOR TOPPING
(Clauses 6.1, 6.2 and 7.1 to 7.3)
SL TYPE OF FLOOR THICKNESS OF GRANO- REMARKS
No. TOPPING LITHE CONCRETE
IN mm, Mifl
A. Flow Topping Laid Over Base Concrete on Ground
1. Floor topping laid monolithi- 20 Granolithic concrete floor top-
tally with the base concrete ping shall be laid monolithic
with the base concrete
2. Floor topping laid separately
on hardened base concrete
‘HJ Granolithic concrete floor top-
ping shall be laid separately
over specially prepared surface
of set and hardened base con-
b. Floor Topping hid Over Suspended Slabs
3. Floor topping laid monolithi- 20 The granolithic concrete topping
tally with the suspended shall be laid and finished
slab monolithic with the suspended
concrete of the suspended slab
has stiffened enough ( but is
still green ) to allow the work-
men to tread over it by plac-
4. Floor topping laid over the
hardened suspended slab
40 The topping shall be laid sepa-
rately over the specially pre-
pared surface of set and
hardened suspended slab
405. Floor topping laid over
Cushioning layer of lime con-
Crete of 40 to 50 mm thickness
shall be laid over the prepared
surface of suspended slab.
Granolithic concrete topping
shall be laid as in 4
IS : 5491- 1969
8.1 Immediately after the flooring surface is finished it shall be protected
from rapid drying, by erecting barriers against wind or draught and
strong sunlight. As soon as the surface had hardened sufficiently to
prevent damage to it, it shall be kept continuously moist for at least ten
days by means of wet gunny bags, 50 mm thick layer of damp sand spread
over the surface or pooling water on the surface. During this period the
flooring shall not be exposed to any traffic. Premature exposure to traffic
will lead to damage to the surface which cannot be satisfactorily
9.1 The work should be inspected during progress and after completion,
special attention being paid to the following points:
a) Preparation of the base, where the floor finish is laid separately;
b) Proper compaction;
c) Correct finishing; and
d) Correct curing.
10. MAINTENANCE .
10.1 Except where oil and grease are likely to be spilt frequent washing of
the surface with water may be sufficient to maintain the floor finish in
a clean condition. Grease stains may be removed by means of sodium
metasilicate, caustic soda, some phosphates or other proprietary materials.
( Clause 3.6 )
SURFACE TREATMENT TO GRANOLITHIC CONCRETE
A-l.1 It is not necessary, generally, to apply any further treatment to the
granolithic cancrete floor top surface, but dusting may be reduced by the
application of one of the surface hardening solutions described in 3.6.
These treatments are likely to need renewal at intervals of one year.
Where proprietory materials are to be used, advice should be obtained from
IS : 5491-1969
A-2. CLEANING THE SURFACE
A-2.1 The top surface of the granolithic concrete should be clean and free
from grease or oil to enable the hardening solutions to penetrate. Sweep-
ing to remove dust and dirt may be adequate only in some cases
of new floors and additional cleaning may be necessary. The top surface
shall be wetted with water and scrubbed with coir or steel wire brush and
thoroughly cleaned by washing with clean water. The floor should
be allowed to dry so that the hardening solution can be absorbc:d into the
A-3.1 Sodium Silicate-A solution containing one part by volume of
sodium silicate and four to six parts of water should be spread cvcnly over
the granolithic concrete top surface with a mop or soft brush, the stronger
solution being used on a less absorptive surface. Any excess material
should be wiped off and the floor allowed to dry. After the floor has
been washed with clean water, a second coat, containing one part ol
sodium silicate to three or four parts of water, should be applied, and this
should be allowed to. dry similarly. A third coat may be applied after
washing if the floor is still porous. After drying, the flock should be
washed with hot’ clean water. Effective results are obtained if the
treatment is applied seven to ten days after the end of.curing.
A-3.2 Silicofluoride - The cr~ta% of magnesium silicofluoricle or of zinc
silicofluoride should be d&solved in water at the rate of O-1 g/cm” for the
&st coat and 0.2 g/cm3 for subsequent coats. Three coats are usually
applied at 24-hour intqrvals. There is no need to wash the top surface
of the floor between coats, but it is advisable to wash with clean water
after the final treatment.
BUREAU QF INDIAN STANDARDS
Manak Bhavan, 9 Bahadur Shah Zafar Marg, NEW DELHI 110002
Telephones: 331 01 31, 331 13.76 Telegrams: Manaksanstha
( Common to all Offices )
Regional Offices: Telephone
Central : Manak Bhavan, 9 Bahadur Shah Zafar Marg,
331 01 31
NEW DELHI 110002 331 1375
*Eastern : l/l 4 C. I. T. Scheme VII M, V. I. P. Road, 36 24 99
Maniktola. CALCUTTA 700054
Northern : SC0 445-446, Sector 35-C,
Southern : C. I. T. Campus, MADRAS 600113
3 16 41
41 24 42
41 25 19
twestern : Manakalava. E9 MIDC. Marol, Andheri ( East 1. 6 32 92 95a- -- -
#Pushpak’. Nurmohamed Shaikh Marg, Kharlpur,
SPeenya Industrial Area 1st Stage, Bangalore Tumkur Road
Gangotri Complex, 5th Floor, Bhadbhada Road, T. T. Nagar,
Plot No. 82/83. Lewis Road. BHUBANESHWAR 751002
531’5. Ward No. 29, R.G. Barua Road, 5th Byelane,
5-8-56C L. N. Gupta Marg ( Nampally Station Road ),
R14 Yudhister Marg. C Scheme, JAIPUR 302005
117/418 B Sarvodaya Nagar, KANPUR 208005
Fjatliputra Industrial Estate, PATNA 809013
T.C. No. 14/1421. Universitv P.O.. Palayam
inspection Offices ( With Sale Point ):
2 51 71Pwshpanjali, First Floor, 205-A West High Court Road,
Shankar Nagar Square, NAGPUR 440010
Institution of-Engineers ( India ) Building,.l332 Shivaji Nagar, 5 24 35
2 63 48
2 63 49
38 49 55
38 49 56
5 36 27
3 31 77
6 34 71
6 98 32
21 68 76
21 82 92
6 23 05
16 21 04
lSales’Office in Calcutta is at 5 Chowringhee Approach, P. 0. Princep 27 68 00
Street. Calcutta 700072
tSales Office in Bombay is at Novelty Chambers, Grant Road, 89 65 28
ISales Office in Bangalore is at Unity Building, Narasimharaja Square, 22 36 71
Reprography Unit, BIS,’ New Delhi, Indi‘a-. ‘i’
r -- ._